<p>Great material but very hard to print as it does not stick easy to the build plate as it has a low friction coefficient to grip onto the heated bed. Also, the material sets quite fast, once the filament leaves the nozzle, it soon hardens so you need to be careful with retraction and Z-hop (leaving small peaks that will be hit later by the nozzle knocking over your print). </p>

<p>My experience with printing this material is based on printing with an Ultimaker 3 Extended (on glass) using a modified material profile (based on Nylon). It is printed at 240 °C (+5 °C for the first layer), no usage of the part cooling fan (if you do use cooling, the layers will not adhere well), a heated bed temperature of 80 °C, and a slow printing speed of 40 mm/s (20 mm/s for the first and second layer).</p>

<p><em>Ultimaker 3 Extended with printed POM bearing:</em></p>

<p><a href="https://i.sstatic.net/bznZ5.jpg" rel="noreferrer"><img src="https://i.sstatic.net/bznZ5.jpg" alt="Ultimaker 3 Extended with printed POM bearing"></a></p>

<p>First thing I learned is to use quite large brim's (the image above shows a rather small one for this short bearing, for the longer bearings the brim size was more than doubled, e.g. 20 mm), brims enlarge the surface area so that there is more material that grabs hold of the heated bed. Also ensure to get it to stick long enough is heating the bed to 80 °C after smearing ABS juice (ABS dissolved in acetone) and spraying a <a href="https://en.wikipedia.org/wiki/Polyvinyl_alcohol" rel="noreferrer">PVA</a> based spray over the dried ABS juice layer (3DLAC has been used, but other hairsprays or even gluesticks may work as well, as long as there is PVA in it). The temperature of 80 °C is chosen as this is the temperature where my PVA spray has the most tack/sticky-ness.</p>

<p>Other solutions like heating the bed up to 110 °C using 3DLAC or specifically designed sprays for higher temperature like e.g. Dimafix did not work well for me.</p>

<p>Note that complete infill may also give problems as filling out the whole surface area sometimes creates excess material that curls up, which is an easy target to be hit by the nozzle on the next layer. </p>

<p><em>This image shows an <a href="https://www.thingiverse.com/thing:2476782" rel="noreferrer">example</a> of using the printed customized igus® POM bearing that is as long as the mount height:</em></p>

<p><a href="https://i.sstatic.net/HXXJE.jpg" rel="noreferrer"><img src="https://i.sstatic.net/HXXJE.jpg" alt="Prusa clone X-axis mount with inserted custom bearing"></a></p>

<p><em>Collection of POM printed bearings:</em></p>

<p><a href="https://i.sstatic.net/HpCBE.jpg" rel="noreferrer"><img src="https://i.sstatic.net/HpCBE.jpg" alt="Collection of POM printed bearings"></a></p>

<p><em>Another <a href="https://www.thingiverse.com/thing:2520976" rel="noreferrer">application</a> of POM bearings:</em></p>

<p><a href="https://i.sstatic.net/4B6Dn.jpg" rel="noreferrer"><img src="https://i.sstatic.net/4B6Dn.jpg" alt="Bowden E3D mount"></a></p>

<p><em>CoreXY hot end carriage</em></p>

<p><a href="https://i.sstatic.net/s0Sq2.jpg" rel="noreferrer"><img src="https://i.sstatic.net/s0Sq2.jpg" alt="Hypercube Evolution hot end carriage"></a><a href="https://i.sstatic.net/IFtkN.jpg" rel="noreferrer"><img src="https://i.sstatic.net/IFtkN.jpg" alt="Hypercube Evolution X-Y mount bearing"></a></p>

CC BY-SA 4.0
2018-07-06T11:30:53.763Z
2018-07-11T07:32:00.157Z
2018-07-11T07:32:00.157Z
0scar
<p>In the creation of the process of printing my own bearings to reduce noise, minimize play/tolerances and size the bearings to the actual size of the application, I obtained a spool of <a href="https://en.wikipedia.org/wiki/Polyoxymethylene" rel="nofollow noreferrer">Polyoxymethylene</a> (POM) or also known as Acetal or Delrin.</p>
<p><a href="https://i.sstatic.net/erVOB.jpg" rel="nofollow noreferrer"><img src="https://i.sstatic.net/erVOB.jpg" alt="Spool of POM filament" /></a></p>
<p>This polymer is a thermoplastic polymer that is frequently used in engineering precision parts that require high stiffness, low friction and dimensional stability. It has been chosen for these material properties to be used as bearing material for linear guide rails.</p>
<p><em>This image shows an example of the <a href="https://www.printables.com/model/832136-parametric-igus-style-linear-bearing-rjmp-01-xx-an" rel="nofollow noreferrer">application</a> of customized igus® bearing that is as long as the housing part it is going to fit in:</em>
<a href="https://i.sstatic.net/QnKHc.jpg" rel="nofollow noreferrer"><img src="https://i.sstatic.net/QnKHc.jpg" alt="customized igus® bearing" /></a></p>
<p>Prints frequently get knocked over as it does not stick well.</p>
<p>How do I get POM filament to stick to the build plate?</p>

CC BY-SA 4.0
2018-12-09T16:35:19.413Z
Any comments on success/failure on this?
I tried:
1. plain heatbed = bad adhesion, zero
2. blue tape = better but peels off
3. blue tape and glustick = peels off after 1 or 2 layers tried both low and high bed temperature and on/off fan in all combinations,
without a success :(
Miro Krsjak
CC BY-SA 4.0
2018-12-10T10:14:30.780Z
@MiroKrsjak As described in the answer, I get very good adhesion with 3DLAC/ABS juice and a large brim. Lately I even do not use ABS juice anymore, only PVA based spray glue (3DLAC). Works fine for me.
0scar
CC BY-SA 4.0
2019-02-14T19:54:45.027Z
Wow, first time I hear about printing Delrin, it opens up a whole world of possibilities. Just ordered a spool, I'll definitely try to print it using DustNPrint, so far it has proven very good with abs, pp, pc, nylon and all the easy ones like pla and petg. I'll be posting my results asap.
MSteve
<filament><heated-bed><adhesion><pom>
POM filament not sticking to the build plate?
0scar
# POM filament not sticking to the build plate?

(Asked by: username_0 on 2018-07-06)

In the creation of the process of printing my own bearings to reduce noise, minimize play/tolerances and size the bearings to the actual size of the application, I obtained a spool of [Polyoxymethylene](https://en.wikipedia.org/wiki/Polyoxymethylene) (POM) or also known as Acetal or Delrin.

[![Spool of POM filament](https://i.sstatic.net/erVOB.jpg)](https://i.sstatic.net/erVOB.jpg)

This polymer is a thermoplastic polymer that is frequently used in engineering precision parts that require high stiffness, low friction and dimensional stability. It has been chosen for these material properties to be used as bearing material for linear guide rails.

*This image shows an example of the [application](https://www.printables.com/model/832136-parametric-igus-style-linear-bearing-rjmp-01-xx-an) of customized igus® bearing that is as long as the housing part it is going to fit in:*
[![customized igus® bearing](https://i.sstatic.net/QnKHc.jpg)](https://i.sstatic.net/QnKHc.jpg)

Prints frequently get knocked over as it does not stick well.

How do I get POM filament to stick to the build plate?

**Tags:** filament, heated-bed, adhesion, pom

> **Comments:**
> **username_1**: Any comments on success/failure on this? I tried: 1. plain heatbed = bad adhesion, zero 2. blue tape = better but peels off 3. blue tape and glustick = peels off after 1 or 2 layers tried both low and high bed temperature and on/off fan in all combinations, without a success :(  
> **username_0**: @username_1 As described in the answer, I get very good adhesion with 3DLAC/ABS juice and a large brim. Lately I even do not use ABS juice anymore, only PVA based spray glue (3DLAC). Works fine for me.  
> **username_2**: Wow, first time I hear about printing Delrin, it opens up a whole world of possibilities. Just ordered a spool, I'll definitely try to print it using DustNPrint, so far it has proven very good with abs, pp, pc, nylon and all the easy ones like pla and petg. I'll be posting my results asap.  

---

## 1 answers

### Answer by username_0 on 2018-07-06. Score: 13 | Accepted answer

Great material but very hard to print as it does not stick easy to the build plate as it has a low friction coefficient to grip onto the heated bed. Also, the material sets quite fast, once the filament leaves the nozzle, it soon hardens so you need to be careful with retraction and Z-hop (leaving small peaks that will be hit later by the nozzle knocking over your print).

My experience with printing this material is based on printing with an Ultimaker 3 Extended (on glass) using a modified material profile (based on Nylon). It is printed at 240 °C (+5 °C for the first layer), no usage of the part cooling fan (if you do use cooling, the layers will not adhere well), a heated bed temperature of 80 °C, and a slow printing speed of 40 mm/s (20 mm/s for the first and second layer).

*Ultimaker 3 Extended with printed POM bearing:*

[![Ultimaker 3 Extended with printed POM bearing](https://i.sstatic.net/bznZ5.jpg)](https://i.sstatic.net/bznZ5.jpg)

First thing I learned is to use quite large brim's (the image above shows a rather small one for this short bearing, for the longer bearings the brim size was more than doubled, e.g. 20 mm), brims enlarge the surface area so that there is more material that grabs hold of the heated bed. Also ensure to get it to stick long enough is heating the bed to 80 °C after smearing ABS juice (ABS dissolved in acetone) and spraying a [PVA](https://en.wikipedia.org/wiki/Polyvinyl_alcohol) based spray over the dried ABS juice layer (3DLAC has been used, but other hairsprays or even gluesticks may work as well, as long as there is PVA in it). The temperature of 80 °C is chosen as this is the temperature where my PVA spray has the most tack/sticky-ness.

Other solutions like heating the bed up to 110 °C using 3DLAC or specifically designed sprays for higher temperature like e.g. Dimafix did not work well for me.

Note that complete infill may also give problems as filling out the whole surface area sometimes creates excess material that curls up, which is an easy target to be hit by the nozzle on the next layer.

*This image shows an [example](https://www.thingiverse.com/thing:2476782) of using the printed customized igus® POM bearing that is as long as the mount height:*

[![Prusa clone X-axis mount with inserted custom bearing](https://i.sstatic.net/HXXJE.jpg)](https://i.sstatic.net/HXXJE.jpg)

*Collection of POM printed bearings:*

[![Collection of POM printed bearings](https://i.sstatic.net/HpCBE.jpg)](https://i.sstatic.net/HpCBE.jpg)

*Another [application](https://www.thingiverse.com/thing:2520976) of POM bearings:*

[![Bowden E3D mount](https://i.sstatic.net/4B6Dn.jpg)](https://i.sstatic.net/4B6Dn.jpg)

*CoreXY hot end carriage*

[![Hypercube Evolution hot end carriage](https://i.sstatic.net/s0Sq2.jpg)](https://i.sstatic.net/s0Sq2.jpg)[![Hypercube Evolution X-Y mount bearing](https://i.sstatic.net/IFtkN.jpg)](https://i.sstatic.net/IFtkN.jpg)


---

